LMucko/crystallography-open-database huggingface dataset:
New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid Solution Phosphors and Its Luminescence Properties
Jun Zhou; Zhiguo Xia; Mingyue Chen; Maxim S. Molokeev; Quanlin Liu; Scientific Reports 5 (2015) 12149–12153; doi:10.1038/srep12149

data_1529494
_publ_section_title
;
 New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid
 Solution Phosphors and Its Luminescence Properties
;
_journal_issue                   0
_journal_name_full               'Scientific Reports'
_journal_page_first              12149
_journal_page_last               12153
_journal_paper_doi               10.1038/srep12149
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Al8.51 Mg4 O36 Si9.49, 0.13(K4)'
_chemical_formula_sum            'Al8.51 K0.52 Mg4 O36 Si9.49'
_chemical_formula_weight         1189.74
_space_group_IT_number           192
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2c'
_symmetry_space_group_name_H-M   'P 6/m c c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.79423(48)
_cell_length_b                   9.79423(48)
_cell_length_c                   9.34129(51)
_cell_measurement_temperature    300
_cell_volume                     776.03(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    8.936
_exptl_crystal_density_diffrn    2.546
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0202545905
_pd_meas_2theta_range_max        120.007591
_pd_meas_2theta_range_min        5.0020266
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 8 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.212
_pd_proc_ls_prof_wR_expected     2.853
_pd_proc_ls_prof_wR_factor       7.636
_pd_proc_number_of_points        5678
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   2.676
_refine_ls_R_I_factor            1.88
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            K0p26Mg2Al4p26Si4p74O18_Eu.cif
_cod_data_source_block           a
_cod_original_cell_volume        776.029(87)
_cod_original_sg_symbol_Hall
;
-P 6 2c
;
_cod_original_sg_symbol_H-M      P6/mcc
_cod_original_formula_sum
;
Al8.51 K0.52 Mg4 O36 Si9.49
;
_cod_database_code               1529494
_cod_database_fobs_code          1529494
New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid Solution Phosphors and Its Luminescence Properties
Jun Zhou; Zhiguo Xia; Mingyue Chen; Maxim S. Molokeev; Quanlin Liu; Scientific Reports 5 (2015) 12149–12153; doi:10.1038/srep12149

data_1529495
_publ_section_title
;
 New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid
 Solution Phosphors and Its Luminescence Properties
;
_journal_issue                   0
_journal_name_full               'Scientific Reports'
_journal_page_first              12149
_journal_page_last               12153
_journal_paper_doi               10.1038/srep12149
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Al9 Mg4 O36 Si9, K'
_chemical_formula_sum            'Al9 K Mg4 O36 Si9'
_chemical_formula_weight         1207.97
_space_group_IT_number           192
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2c'
_symmetry_space_group_name_H-M   'P 6/m c c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.79964(49)
_cell_length_b                   9.79964(49)
_cell_length_c                   9.36376(55)
_cell_measurement_temperature    300
_cell_volume                     778.76(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    9.437
_exptl_crystal_density_diffrn    2.576
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        120.007591
_pd_meas_2theta_range_min        5.0020266
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 6 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.758
_pd_proc_ls_prof_wR_expected     2.907
_pd_proc_ls_prof_wR_factor       8.438
_pd_proc_number_of_points        5750.27822
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   2.903
_refine_ls_R_I_factor            2.35
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            K0p5Mg2Al4p5Si4p5O18_Eu.cif
_cod_data_source_block           a
_cod_original_cell_volume        778.756(90)
_cod_original_sg_symbol_Hall
;
-P 6 2c
;
_cod_original_sg_symbol_H-M      P6/mcc
_cod_original_formula_sum
;
Al9 K Mg4 O36 Si9
;
_cod_database_code               1529495
_cod_database_fobs_code          1529495
New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid Solution Phosphors and Its Luminescence Properties
Jun Zhou; Zhiguo Xia; Mingyue Chen; Maxim S. Molokeev; Quanlin Liu; Scientific Reports 5 (2015) 12149–12153; doi:10.1038/srep12149

data_1529496
_publ_section_title
;
 New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid
 Solution Phosphors and Its Luminescence Properties
;
_journal_issue                   0
_journal_name_full               'Scientific Reports'
_journal_page_first              12149
_journal_page_last               12153
_journal_paper_doi               10.1038/srep12149
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Al9.02 Mg4 O36 Si8.98, 0.247(Rb4)'
_chemical_formula_sum            'Al9.02 Mg4 O36 Rb0.99 Si8.98'
_chemical_formula_weight         1253.29
_space_group_IT_number           192
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2c'
_symmetry_space_group_name_H-M   'P 6/m c c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.79552(26)
_cell_length_b                   9.79552(26)
_cell_length_c                   9.37418(32)
_cell_measurement_temperature    300
_cell_volume                     778.97(4)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    10.107
_exptl_crystal_density_diffrn    2.671
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        120.007591
_pd_meas_2theta_range_min        5.0020266
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 6 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.553
_pd_proc_ls_prof_wR_expected     3.271
_pd_proc_ls_prof_wR_factor       6.062
_pd_proc_number_of_points        5750.27822
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.854
_refine_ls_R_I_factor            1.379
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Rb0p17Mg2Al4p17Si4p83O18_Eu.cif
_cod_data_source_block           a
_cod_original_cell_volume        778.967(49)
_cod_original_sg_symbol_Hall
;
-P 6 2c
;
_cod_original_sg_symbol_H-M      P6/mcc
_cod_original_formula_sum
;
Al9.02 Mg4 O36 Rb0.99 Si8.98
;
_cod_database_code               1529496
_cod_database_fobs_code          1529496
New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid Solution Phosphors and Its Luminescence Properties
Jun Zhou; Zhiguo Xia; Mingyue Chen; Maxim S. Molokeev; Quanlin Liu; Scientific Reports 5 (2015) 12149–12153; doi:10.1038/srep12149

data_1529497
_publ_section_title
;
 New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid
 Solution Phosphors and Its Luminescence Properties
;
_journal_issue                   0
_journal_name_full               'Scientific Reports'
_journal_page_first              12149
_journal_page_last               12153
_journal_paper_doi               10.1038/srep12149
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Al8.51 Mg4 O36 Si9.49, 0.13(Rb4)'
_chemical_formula_sum            'Al8.51 Mg4 O36 Rb0.52 Si9.49'
_chemical_formula_weight         1213.85
_space_group_IT_number           192
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2c'
_symmetry_space_group_name_H-M   'P 6/m c c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.79723(44)
_cell_length_b                   9.79723(44)
_cell_length_c                   9.34351(54)
_cell_measurement_temperature    300
_cell_volume                     776.69(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    9.290
_exptl_crystal_density_diffrn    2.595
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0202545905
_pd_meas_2theta_range_max        120.007591
_pd_meas_2theta_range_min        5.0020266
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.880
_pd_proc_ls_prof_wR_expected     2.725
_pd_proc_ls_prof_wR_factor       6.528
_pd_proc_number_of_points        5678
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   2.395
_refine_ls_R_I_factor            2.78
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Rb0p26Mg2Al4p26Si4p74O18_Eu.cif
_cod_data_source_block           a
_cod_original_cell_volume        776.689(83)
_cod_original_sg_symbol_Hall
;
-P 6 2c
;
_cod_original_sg_symbol_H-M      P6/mcc
_cod_original_formula_sum
;
Al8.51 Mg4 O36 Rb0.52 Si9.49
;
_cod_database_code               1529497
_cod_database_fobs_code          1529497
New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid Solution Phosphors and Its Luminescence Properties
Jun Zhou; Zhiguo Xia; Mingyue Chen; Maxim S. Molokeev; Quanlin Liu; Scientific Reports 5 (2015) 12149–12153; doi:10.1038/srep12149

data_1529498
_publ_section_title
;
 New Insight into Phase Formation of MxMg2Al4+xSi5-xO18:Eu2+ Solid
 Solution Phosphors and Its Luminescence Properties
;
_journal_issue                   0
_journal_name_full               'Scientific Reports'
_journal_page_first              12149
_journal_page_last               12153
_journal_paper_doi               10.1038/srep12149
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety         'Al9 Mg4 O36 Si9, Rb'
_chemical_formula_sum            'Al9 Mg4 O36 Rb Si9'
_chemical_formula_weight         1254.34
_space_group_IT_number           192
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6 2c'
_symmetry_space_group_name_H-M   'P 6/m c c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.79795(40)
_cell_length_b                   9.79795(40)
_cell_length_c                   9.36370(51)
_cell_measurement_temperature    300
_cell_volume                     778.48(6)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    10.134
_exptl_crystal_density_diffrn    2.676
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        120.007591
_pd_meas_2theta_range_min        5.0020266
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 6 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.300
_pd_proc_ls_prof_wR_expected     2.767
_pd_proc_ls_prof_wR_factor       7.708
_pd_proc_number_of_points        5750.27822
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   2.786
_refine_ls_R_I_factor            2.57
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Rb0p5Mg2Al4p5Si4p5O18_Eu.cif
_cod_data_source_block           a
_cod_original_cell_volume        778.482(77)
_cod_original_sg_symbol_Hall
;
-P 6 2c
;
_cod_original_sg_symbol_H-M      P6/mcc
_cod_original_formula_sum
;
Al9 Mg4 O36 Rb Si9
;
_cod_database_code               1529498
_cod_database_fobs_code          1529498
Preparation, Structure and Up-conversion Luminescence of Yb3+/Er3+ co-doped SrIn2O4 Phosphors
Ming Guan; Hong Zheng; Lefu Mei; Maxim S. Molokeev; Jing Xie; Tao Yang; Xiaowen Wu; Saifang Huang; Zhaohui Huang; Journal of the American Ceramic Society 98 (2015) 1182–1187; doi:10.1111/jace.13415

data_1529499
_publ_section_title
;
 Preparation, Structure and Up-conversion Luminescence of Yb3+/Er3+
 co-doped SrIn2O4 Phosphors
;
_journal_issue                   4
_journal_name_full               'Journal of the American Ceramic Society'
_journal_page_first              1182
_journal_page_last               1187
_journal_paper_doi               10.1111/jace.13415
_journal_volume                  98
_journal_year                    2015
_chemical_formula_moiety         'Er0.04 In7.96 O16, 4(Sr)'
_chemical_formula_sum            'Er0.04 In7.96 O16 Sr4'
_chemical_formula_weight         1527.14
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.83173(14)
_cell_length_b                   3.266226(48)
_cell_length_c                   11.49502(18)
_cell_measurement_temperature    300
_cell_volume                     369.136(10)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    116.632
_exptl_crystal_density_diffrn    6.9080(11)
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        100
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        6.119
_pd_proc_ls_prof_wR_expected     6.758
_pd_proc_ls_prof_wR_factor       9.612
_pd_proc_number_of_points        4750
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.422
_refine_ls_R_I_factor            2.67
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            SrIn2O4_0p01Er.cif
_cod_data_source_block           a
_cod_original_cell_volume        369.1355(95)
_cod_original_sg_symbol_Hall
;
-P 2ac 2n
;
_cod_original_sg_symbol_H-M      Pnma
_cod_original_formula_sum
;
Er0.04 In7.96 O16 Sr4
;
_cod_database_code               1529499
_cod_database_fobs_code          1529499
Preparation, Structure and Up-conversion Luminescence of Yb3+/Er3+ co-doped SrIn2O4 Phosphors
Ming Guan; Hong Zheng; Lefu Mei; Maxim S. Molokeev; Jing Xie; Tao Yang; Xiaowen Wu; Saifang Huang; Zhaohui Huang; Journal of the American Ceramic Society 98 (2015) 1182–1187; doi:10.1111/jace.13415

data_1529500
_publ_section_title
;
 Preparation, Structure and Up-conversion Luminescence of Yb3+/Er3+
 co-doped SrIn2O4 Phosphors
;
_journal_issue                   4
_journal_name_full               'Journal of the American Ceramic Society'
_journal_page_first              1182
_journal_page_last               1187
_journal_paper_doi               10.1111/jace.13415
_journal_volume                  98
_journal_year                    2015
_chemical_formula_moiety         'Er0.04 In7.56 O16 Yb0.40, 4(Sr)'
_chemical_formula_sum            'Er0.04 In7.56 O16 Sr4 Yb0.4'
_chemical_formula_weight         1550.43
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.85272(11)
_cell_length_b                   3.274175(38)
_cell_length_c                   11.52212(13)
_cell_measurement_temperature    300
_cell_volume                     371.698(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    115.395
_exptl_crystal_density_diffrn    6.926348
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        100
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 4 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.968
_pd_proc_ls_prof_wR_expected     6.654
_pd_proc_ls_prof_wR_factor       7.028
_pd_proc_number_of_points        4750
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.056
_refine_ls_R_I_factor            1.73
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            SrIn2O4_0p1Yb_0p01Er.cif
_cod_data_source_block           a
_cod_original_cell_volume        371.6982(74)
_cod_original_sg_symbol_Hall
;
-P 2ac 2n
;
_cod_original_sg_symbol_H-M      Pnma
_cod_original_formula_sum
;
Er0.04 In7.56 O16 Sr4 Yb0.40
;
_cod_database_code               1529500
_cod_database_fobs_code          1529500
Ca/Sr ratio dependent structure and up-conversion luminescence of (Ca1-xSrx)In2O4: Yb3+/Ho3+ phosphors
Ming Guan; Hong Zheng; Zhaohui Huang; Bin Ma; Maxim S. Molokeev; Saifang Huang; Lefu Mei; RSC Advances 5 (2015) 59403–59407; doi:10.1039/C5RA08467A

data_7221947
_publ_section_title
;
 Ca/Sr ratio dependent structure and up-conversion luminescence of
 (Ca1-xSrx)In2O4: Yb3+/Ho3+ phosphors
;
_journal_issue                   73
_journal_name_full               'RSC Advances'
_journal_page_first              59403
_journal_page_last               59407
_journal_paper_doi               10.1039/C5RA08467A
_journal_volume                  5
_journal_year                    2015
_chemical_formula_moiety
'Ho0.02 In7.40 O16 Yb0.40, 4(Sr0.10), 3.6(Ca)'
_chemical_formula_sum            'Ca3.6 Ho0.02 In7.4 O16 Sr0.4 Yb0.4'
_chemical_formula_weight         1358.18
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.67494(49)
_cell_length_b                   3.22534(17)
_cell_length_c                   11.33068(50)
_cell_measurement_temperature    300
_cell_volume                     353.57(3)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    113.159
_exptl_crystal_density_diffrn    6.379
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0160352
_pd_meas_2theta_range_max        120.004454
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        8.535
_pd_proc_ls_prof_wR_expected     6.139
_pd_proc_ls_prof_wR_factor       11.071
_pd_proc_number_of_points        7172
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.803
_refine_ls_R_I_factor            3.13
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Ca0p9Sr0p1In2O4_0p005Ho_0p1Yb.cif
_cod_data_source_block           a
_cod_original_cell_volume        353.574(30)
_cod_original_sg_symbol_Hall
;
-P 2ac 2n
;
_cod_original_sg_symbol_H-M      Pnma
_cod_original_formula_sum
;
Ca3.60 Ho0.02 In7.40 O16 Sr0.40 Yb0.40
;
_cod_database_code               7221947
_cod_database_fobs_code          7221947